General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.9 - 7.93 g/cm³ Show Material materials with Density of 7.9 - 7.93 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | -100.0 °C | 206 GPa Show Material materials with Elastic modulus of 206 GPa |

20.0 °C | 196 - 200 GPa Show Material materials with Elastic modulus of 196 - 200 GPa | |

95.0 °C | 193.05 GPa Show Material materials with Elastic modulus of 193.05 GPa | |

100.0 °C | 190 - 194 GPa Show Material materials with Elastic modulus of 190 - 194 GPa | |

150.0 °C | 188.23 GPa Show Material materials with Elastic modulus of 188.23 GPa | |

200.0 °C | 182 - 186 GPa Show Material materials with Elastic modulus of 182 - 186 GPa | |

205.0 °C | 182.71 GPa Show Material materials with Elastic modulus of 182.71 GPa | |

260.0 °C | 177.88 GPa Show Material materials with Elastic modulus of 177.88 GPa | |

300.0 °C | 174 - 179 GPa Show Material materials with Elastic modulus of 174 - 179 GPa | |

315.0 °C | 174.44 GPa Show Material materials with Elastic modulus of 174.44 GPa | |

370.0 °C | 168.92 GPa Show Material materials with Elastic modulus of 168.92 GPa | |

400.0 °C | 166 - 172 GPa Show Material materials with Elastic modulus of 166 - 172 GPa | |

425.0 °C | 164.1 GPa Show Material materials with Elastic modulus of 164.1 GPa | |

485.0 °C | 159.96 GPa Show Material materials with Elastic modulus of 159.96 GPa | |

500.0 °C | 158 - 165 GPa Show Material materials with Elastic modulus of 158 - 165 GPa | |

540.0 °C | 155.13 GPa Show Material materials with Elastic modulus of 155.13 GPa | |

595.0 °C | 151 GPa Show Material materials with Elastic modulus of 151 GPa | |

600.0 °C | 150 GPa Show Material materials with Elastic modulus of 150 GPa | |

650.0 °C | 146.17 GPa Show Material materials with Elastic modulus of 146.17 GPa | |

700.0 °C | 142 GPa Show Material materials with Elastic modulus of 142 GPa | |

705.0 °C | 140.65 GPa Show Material materials with Elastic modulus of 140.65 GPa | |

760.0 °C | 135.83 GPa Show Material materials with Elastic modulus of 135.83 GPa | |

800.0 °C | 134 GPa Show Material materials with Elastic modulus of 134 GPa | |

815.0 °C | 131.69 GPa Show Material materials with Elastic modulus of 131.69 GPa | |

900.0 °C | 127 GPa Show Material materials with Elastic modulus of 127 GPa | |

1000.0 °C | 120 GPa Show Material materials with Elastic modulus of 120 GPa | |

Elongation | 20.0 °C | 20 % Show Material materials with Elongation of 20 % |

Poisson's ratio | 20.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] |

95.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

150.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

205.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

260.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

315.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

370.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

425.0 °C | 0.31 [-] Show Material materials with Poisson's ratio of 0.31 [-] | |

485.0 °C | 0.32 [-] Show Material materials with Poisson's ratio of 0.32 [-] | |

540.0 °C | 0.32 [-] Show Material materials with Poisson's ratio of 0.32 [-] | |

595.0 °C | 0.34 [-] Show Material materials with Poisson's ratio of 0.34 [-] | |

650.0 °C | 0.34 [-] Show Material materials with Poisson's ratio of 0.34 [-] | |

705.0 °C | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | |

760.0 °C | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | |

815.0 °C | 0.35 [-] Show Material materials with Poisson's ratio of 0.35 [-] | |

Unlock all property charts | ||

Shear modulus | 20.0 °C | 77.22 GPa Show Material materials with Shear modulus of 77.22 GPa |

95.0 °C | 74.46 GPa Show Material materials with Shear modulus of 74.46 GPa | |

150.0 °C | 73.08 GPa Show Material materials with Shear modulus of 73.08 GPa | |

205.0 °C | 71.02 GPa Show Material materials with Shear modulus of 71.02 GPa | |

260.0 °C | 68.26 GPa Show Material materials with Shear modulus of 68.26 GPa | |

315.0 °C | 66.88 GPa Show Material materials with Shear modulus of 66.88 GPa | |

370.0 °C | 64.81 GPa Show Material materials with Shear modulus of 64.81 GPa | |

425.0 °C | 62.74 GPa Show Material materials with Shear modulus of 62.74 GPa | |

485.0 °C | 60.67 GPa Show Material materials with Shear modulus of 60.67 GPa | |

540.0 °C | 58.61 GPa Show Material materials with Shear modulus of 58.61 GPa | |

595.0 °C | 56.54 GPa Show Material materials with Shear modulus of 56.54 GPa | |

650.0 °C | 54.47 GPa Show Material materials with Shear modulus of 54.47 GPa | |

705.0 °C | 53.09 GPa Show Material materials with Shear modulus of 53.09 GPa | |

760.0 °C | 51.02 GPa Show Material materials with Shear modulus of 51.02 GPa | |

815.0 °C | 48.95 GPa Show Material materials with Shear modulus of 48.95 GPa | |

Unlock all property charts | ||

Tensile strength | 20.0 °C | 700 - 900 MPa Show Material materials with Tensile strength of 700 - 900 MPa |

Yield strength Rp0.2 | 20.0 °C | 350 MPa Show Material materials with Yield strength Rp0.2 of 350 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | |

20.0 °C | 1.61E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.61E-5 1/K | ||

100.0 °C | 1.6E-5 - 1.67E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.6E-5 - 1.67E-5 1/K | ||

200.0 °C | 1.65E-5 - 1.72E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.65E-5 - 1.72E-5 1/K | ||

300.0 °C | 1.7E-5 - 1.77E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.7E-5 - 1.77E-5 1/K | ||

400.0 °C | 1.75E-5 - 1.81E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.75E-5 - 1.81E-5 1/K | ||

500.0 °C | 1.8E-5 - 1.84E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.8E-5 - 1.84E-5 1/K | ||

600.0 °C | 1.88E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.88E-5 1/K | ||

700.0 °C | 1.91E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.91E-5 1/K | ||

800.0 °C | 1.94E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.94E-5 1/K | ||

900.0 °C | 1.97E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.97E-5 1/K | ||

1000.0 °C | 2E-5 1/K Show Material materials with Coefficient of thermal expansion of 2E-5 1/K | ||

Unlock all property charts | |||

Melting point | 1230 - 1480 °C Show Material materials with Melting point of 1230 - 1480 °C | Typical for Austenitic Stainless Steel | |

Specific heat capacity | -100.0 °C | 440 J/(kg·K) Show Material materials with Specific heat capacity of 440 J/(kg·K) | |

20.0 °C | 472 - 500 J/(kg·K) Show Material materials with Specific heat capacity of 472 - 500 J/(kg·K) | ||

100.0 °C | 487 J/(kg·K) Show Material materials with Specific heat capacity of 487 J/(kg·K) | ||

200.0 °C | 503 J/(kg·K) Show Material materials with Specific heat capacity of 503 J/(kg·K) | ||

300.0 °C | 512 J/(kg·K) Show Material materials with Specific heat capacity of 512 J/(kg·K) | ||

400.0 °C | 520 J/(kg·K) Show Material materials with Specific heat capacity of 520 J/(kg·K) | ||

500.0 °C | 530 J/(kg·K) Show Material materials with Specific heat capacity of 530 J/(kg·K) | ||

600.0 °C | 541 J/(kg·K) Show Material materials with Specific heat capacity of 541 J/(kg·K) | ||

700.0 °C | 551 J/(kg·K) Show Material materials with Specific heat capacity of 551 J/(kg·K) | ||

800.0 °C | 559 J/(kg·K) Show Material materials with Specific heat capacity of 559 J/(kg·K) | ||

900.0 °C | 565 J/(kg·K) Show Material materials with Specific heat capacity of 565 J/(kg·K) | ||

1000.0 °C | 571 J/(kg·K) Show Material materials with Specific heat capacity of 571 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 14.3 - 15 W/(m·K) Show Material materials with Thermal conductivity of 14.3 - 15 W/(m·K) | |

100.0 °C | 15.8 W/(m·K) Show Material materials with Thermal conductivity of 15.8 W/(m·K) | ||

200.0 °C | 17.5 W/(m·K) Show Material materials with Thermal conductivity of 17.5 W/(m·K) | ||

300.0 °C | 19 W/(m·K) Show Material materials with Thermal conductivity of 19 W/(m·K) | ||

400.0 °C | 20.5 W/(m·K) Show Material materials with Thermal conductivity of 20.5 W/(m·K) | ||

500.0 °C | 21.9 W/(m·K) Show Material materials with Thermal conductivity of 21.9 W/(m·K) | ||

600.0 °C | 23.3 W/(m·K) Show Material materials with Thermal conductivity of 23.3 W/(m·K) | ||

700.0 °C | 24.6 W/(m·K) Show Material materials with Thermal conductivity of 24.6 W/(m·K) | ||

800.0 °C | 26 W/(m·K) Show Material materials with Thermal conductivity of 26 W/(m·K) | ||

900.0 °C | 27.4 W/(m·K) Show Material materials with Thermal conductivity of 27.4 W/(m·K) | ||

1000.0 °C | 28.8 W/(m·K) Show Material materials with Thermal conductivity of 28.8 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 3.8 mm²/s Show Material materials with Thermal diffusivity of 3.8 mm²/s | |

100.0 °C | 4 mm²/s Show Material materials with Thermal diffusivity of 4 mm²/s | ||

200.0 °C | 4.2 mm²/s Show Material materials with Thermal diffusivity of 4.2 mm²/s | ||

300.0 °C | 4.6 mm²/s Show Material materials with Thermal diffusivity of 4.6 mm²/s | ||

400.0 °C | 4.8 mm²/s Show Material materials with Thermal diffusivity of 4.8 mm²/s | ||

500.0 °C | 4.9 mm²/s Show Material materials with Thermal diffusivity of 4.9 mm²/s | ||

600.0 °C | 5 mm²/s Show Material materials with Thermal diffusivity of 5 mm²/s | ||

700.0 °C | 5.3 mm²/s Show Material materials with Thermal diffusivity of 5.3 mm²/s | ||

800.0 °C | 5.6 mm²/s Show Material materials with Thermal diffusivity of 5.6 mm²/s | ||

900.0 °C | 5.9 mm²/s Show Material materials with Thermal diffusivity of 5.9 mm²/s | ||

1000.0 °C | 6 mm²/s Show Material materials with Thermal diffusivity of 6 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 7.1E-7 - 7.3E-7 Ω·m Show Material materials with Electrical resistivity of 7.1E-7 - 7.3E-7 Ω·m |

100.0 °C | 7.76E-7 Ω·m Show Material materials with Electrical resistivity of 7.76E-7 Ω·m | |

200.0 °C | 8.49E-7 Ω·m Show Material materials with Electrical resistivity of 8.49E-7 Ω·m | |

300.0 °C | 9.14E-7 Ω·m Show Material materials with Electrical resistivity of 9.14E-7 Ω·m | |

400.0 °C | 9.71E-7 Ω·m Show Material materials with Electrical resistivity of 9.71E-7 Ω·m | |

500.0 °C | 1.02E-6 Ω·m Show Material materials with Electrical resistivity of 1.02E-6 Ω·m | |

600.0 °C | 1.07E-6 Ω·m Show Material materials with Electrical resistivity of 1.07E-6 Ω·m | |

700.0 °C | 1.1E-6 Ω·m Show Material materials with Electrical resistivity of 1.1E-6 Ω·m | |

800.0 °C | 1.14E-6 Ω·m Show Material materials with Electrical resistivity of 1.14E-6 Ω·m | |

900.0 °C | 1.17E-6 Ω·m Show Material materials with Electrical resistivity of 1.17E-6 Ω·m | |

1000.0 °C | 1.19E-6 Ω·m Show Material materials with Electrical resistivity of 1.19E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.08 % Show Material materials with Carbon of 0.08 % |

Chromium | 17 - 19 % Show Material materials with Chromium of 17 - 19 % |

Manganese | 2 % Show Material materials with Manganese of 2 % |

Nickel | 9 - 12 % Show Material materials with Nickel of 9 - 12 % |

Phosphorus | 0.05 % Show Material materials with Phosphorus of 0.05 % |

Silicon | 1 % Show Material materials with Silicon of 1 % |

Sulfur | 0.015 % Show Material materials with Sulfur of 0.015 % |

Titanium | 0.7 % Show Material materials with Titanium of 0.7 % |